- Open Access
Photodegradation and photostabilization of polymers, especially polystyrene: review
© Yousif and Haddad; licensee Springer. 2013
- Received: 23 May 2013
- Accepted: 29 July 2013
- Published: 23 August 2013
Exposure to ultraviolet (UV) radiation may cause the significant degradation of many materials. UV radiation causes photooxidative degradation which results in breaking of the polymer chains, produces free radical and reduces the molecular weight, causing deterioration of mechanical properties and leading to useless materials, after an unpredictable time. Polystyrene (PS), one of the most important material in the modern plastic industry, has been used all over the world, due to its excellent physical properties and low-cost. When polystyrene is subjected to UV irradiation in the presence of air, it undergoes a rapid yellowing and a gradual embrittlement. The mechanism of PS photolysis in the solid state (film) depends on the mobility of free radicals in the polymer matrix and their bimolecular recombination. Free hydrogen radicals diffuse very easily through the polymer matrix and combine in pairs or abstract hydrogen atoms from polymer molecule. Phenyl radical has limited mobility. They may abstract hydrogen from the near surrounding or combine with a polymer radical or with hydrogen radicals. Almost all synthetic polymers require stabilization against adverse environmental effects. It is necessary to find a means to reduce or prevent damage induced by environmental components such as heat, light or oxygen. The photostabilization of polymers may be achieved in many ways. The following stabilizing systems have been developed, which depend on the action of stabilizer: (1) light screeners, (2) UV absorbers, (3) excited-state quenchers, (4) peroxide decomposers, and (5) free radical scavengers; of these, it is generally believed that excited-state quenchers, peroxide decomposers, and free radical scavengers are the most effective. Research into degradation and ageing of polymers is extremely intensive and new materials are being synthesized with a pre-programmed lifetime. New stabilizers are becoming commercially available although their modes of action are sometimes not thoroughly elucidated. They target the many possible ways of polymer degradation: thermolysis, thermooxidation, photolysis, photooxidation, radiolysis etc. With the goal to increase lifetime of a particular polymeric material, two aspects of degradation are of particular importance: Storage conditions, and Addition of appropriate stabilizers. A profound knowledge of degradation mechanisms is needed to achieve the goal.
- Carbon Black
- Chain Scission
- Hinder Amine Light Stabilizer
- Polymer Degradation
- Peroxy Radical
Exposure to ultraviolet (UV) radiation may cause significant degradation of many materials. UV radiation causes photooxidative degradation which results in breaking of the polymer chains, produces radicals and reduces the molecular weight, causing deterioration of mechanical properties and leading to useless materials, after an unpredictable time.
Polystyrene (PS), one of the most important materials from the modern plastic industry, has been used all over the world, due to its excellent physical properties and low-cost. Rabie et al. (2008).
When polystyrene is subjected to UV irradiation in the presence of air, it undergoes a rapid yellowing and a gradual embrittlement Geuskens and David (1975).
The mechanism of PS photolysis in the solid state (film) depends on the mobility of radicals in the polymer matrix and their bimolecular recombination. Hydrogen radicals diffuse very easily through the polymer matrix and combine in pairs or abstract hydrogen atoms from polymer molecule. The phenyl radical has limited mobility. It may abstract hydrogen from the near surrounding or combine with a polymer radical or with hydrogen radicals.
Almost all synthetic polymers require stabilization against adverse environmental effects. It is necessary to find a means to reduce or prevent damage induced by environmental components such as heat, light or oxygen Rabek and Ranby (1974a 1974b).
The photostabilization of polymers may be achieved in many ways. The following stabilizing systems have been developed, which depend on the action of stabilizer: (1) light screeners, (2) UV absorbers, (3) excited-state quenchers, (4) peroxide decomposers, and (5) radical scavengers; of these, it is generally believed that excited-state quenchers, peroxide decomposers, and radical scavengers are the most effective Yousif et al. (2013).
Research into degradation and ageing of polymers is extremely intensive and new materials are being synthesized with a pre-programmed lifetime. New stabilizers are becoming commercially available although their modes of action are sometimes not been thoroughly elucidated. They target the many possible ways of polymer degradation: thermolysis, thermooxidation, photolysis, photooxidation, radiolysis, etc. With the goal for increasing lifetime of a particular polymeric material, two aspects of degradation are of particular importance: storage conditions, and addition of appropriate stabilizers. A profound knowledge of degradation mechanisms is needed to achieve the goal.
Definitions & historical aspects of photodegradation of polymers
Polymers are a broad class of materials which are made from repeating units of smaller molecule called monomers. Polymers can be natural in origin such as the lignin of tree branches. Other polymers are termed synthetic, because they are made by humans from naturally-occurring materials. Example such as polyester and polystyrene. Polymers are useful because of their strength and durability in many applications.
One of the disadvantages of using polymers is that they degrade when they are used in high temperature conditions or in outdoor applications. When polymers are used in outdoor applications, the environment negatively influences the servicelife. This process is called weathering (Zweifel 1998; Wypych 2008).
The term degradation of macromolecules denotes all processes which lead to a decline of polymer properties. It may eventually involve physical processes, such as polymer recrystallization, or denaturation of protein structures. Chemical processes related to degradation may lead to a reduction of average molar mass due to macromolecular chain bond scission or to an increase of molar mass due to crosslinking rendering the polymer insoluble.
The term ageing of polymers is usually associated with long-term changes of polymer properties under the conditions of weathering and may involve any of the above processes Strlic & Kolar (2005).
A wide variety of synthetic and naturally occurring high polymers absorb solar ultraviolet radiation and undergo photolytic, photooxidative, and thermooxidative reactions that result in the degradation of the material (Ayako and Hirose 1999; Scott 2000; Valkoa et al. 2001).
In recent years, the use of polymeric materials has rapidly increased but it is well established that rapid photodegradation of these materials is possible when they are exposed to natural weathering (Guillet 1985; Hamid 2000; Rabek 1996; Bottino et al. 2003). This is a serious issue, with economic and environmental implications and therefore a large effort is focused on understanding the changes that occur at molecular level and the degradation kinetics. Following different routes, UV radiation causes a photooxidative degradation which results in breaking of the polymer chains, produces radical and reduces the molecular weight, causing deterioration of mechanical properties and leading to useless materials, after an unpredictable time (Bottino et al. 2003; Gardella 1988).
Most of the common polymers used in such applications contain photostabilizers to reduce photodamage and to ensure acceptable life times under outdoor exposure conditions.
The use of plastics in building applications is popular in the developing world because of the low cost and the ease of use of plastic components compared to the conventional metal, glass, mortar, wood and other materials. Plastics are used in other products such as outdoor furniture, fishing gear, and marine craft, which are also routinely used outdoors (Andrady 1997; Sampers 2002).
Solar radiation reaching the surface of the earth is characterized by wave lengths from approximately 295 up to 2500 nm. The solar radiation classified as UV-B (280 – 315 nm) has an energy of 426 – 380 KJ mol-1. Fortunately, the higher energetic part of UV-B; 280 – 295 nm, is filtered by the stratosphere and does not reach the earth’s surface, UV-A (315 – 400 nm), has energy between 389 and 300 KJ mol-1 and is less harmful for organic materials than UV-B. Visible (400 – 760 nm). and infrared (760 – 2500nm.) Pospisil and Nespurek (2000).
Photooxidation of organic materials is a major cause of irreversible deterioration for a large number of substances. It is responsible not only for the loss of physical properties of plastics, rubber, but also for foodstuffs Grassie and Scott (1985). In most polymers photooxidative degradation may be induced by UV radiation or catalytic process (or both) and can be accelerated at elevated temperature.
Factors causing the photodegradation
- I)Internal impurities, which may contain chromophoric groups that are introduced into macromolecules during polymerization processing and storage; they include:
Unsaturated bonds (C=C).
Charge–transfer (CT) complexes with oxygen.
- II)External impurities, which may contain chromophoric groups, are:
Traces of solvents, catalyst, …. etc.
Compounds from a polluted urban atmosphere and smog, e.g. polynuclear hydrocarbons such as naphthalene and anthracene in polypropylene and polybutadiene.
Additives (pigments, dyes, thermal stabilizers, photostabilizers, …. etc.).
Traces of metals and metal oxides from processing equipment and containers, such as Fe, Ni or Cr.
Types of polymers degradation
The degradation of polymers usually starts at the outer surface and penetrates gradually into the bulk of the material Blaga (1980).
Polymer degradation can be caused by heat (thermal degradation), light (photodegradation), ionizing radiation (radio degradation), mechanical action, or by fungi, bacteria, yeasts, algae, and their enzymes (biodegradation). The deleterious effects of weathering on polymers generally has been ascribed to a complex set of processes in which the combined action of UV. light and oxygen predominant. The overall light-initiated process in the presence of oxygen generally is referred to as oxidative photodegradation or photooxidation. A pure thermal effect in possible because oxygen is always present and so the process is thermaloxidative degradation Feldman (2002).
There are many different modes of polymer degradation. These are very similar since they all involve chemical reactions that result in bond scission. These modes are: Schnabel (1981).
Chemical degradation refers exclusively to processes, which are induced under the influence of chemical reagent (e.g. acids, bases, solvents reactive gases, etc.) Weidner et al. (1996).
Thermal degradation refers to the case where the polymer, at elevated temperatures, starts to undergo chemical changes without the simultaneous involvement of another compound Guaita et al. (1985).
Biologically initiated degradation also is strongly related to chemical degradation as far as microbial attack is concerned. Microorganisms produce variety of enzymes which are capable of reaction with natural and synthetic polymers Dindar and Icli, (2001).
When polymeric materials are subjected to high energy radiation (e.g. gamma radiation) changes are observed on their molecular structure, mainly chain scission, which leads to reduction in molar mass Vinhas et al. (2003).
Photodegradation is degradation of a photodegradable molecule caused by the absorption of photons, particularly those wavelengths found in sunlight, such as infrared radiation, visible light, and ultraviolet light. However, other forms of electromagnetic radiation can cause photodegradation. Photodegradation includes photodissociation, the breakup of molecules into smaller pieces by photons. It also includes the change of a molecule's shape to make it irreversibly altered, such as the denaturing of proteins, and the addition of other atoms or molecules. A common photodegradation reaction is oxidation. Photodegradation in the environment is part of the process by which ambergris evolves from its fatty precursor. Photodegradation also destroys paintings and other artifacts.
Light - induced polymer degradation, or photodegradation, includes the physical and chemical changes caused by irradiation of polymers with ultraviolet or visible light. In order to be effective, light must be absorbed by the substrate (polymeric system). Thus, the existence of chromophoric groups in the macromolecules is a prerequisite for the initiation of any photochemical reaction Schnabel (1981).
Ketones, quinines, and peroxides are initiators for different reaction degradation or chemical modification occurring in organic compounds Kaczmarek et al. (1999). They absorb light up to about 380 nm, which causes their excitation or cleavage to radicals. One may initiate polymer degradation and other transformation by abstruction of hydrogen atom from a macromolecule (PH) and formation of polymer alkyl radical (P.) (Rabek 1993; Rabek 1996).
The influence of low-molecular weight organic compounds such as benzophenone (BPh), anthraquinone (AQ) and benzoyl peroxide (BPo) on the photoprocesses of polystyrene has been studied. The results indicate that additives accelerate and increase the photodegradation and photooxidation of polystyrene Kaczmarek et al. (1999).
Photodegradation may occur in the absence of oxygen (chain breaking or cross-linking) and the presence of oxygen (photooxidative) degradation. The photooxidative degradation process is induced by UV radiation and other catalysts (or both) and can be accelerated at elevated temperatures.
Photodegradation of polystyrene (e.g. embrittlement and color change) can take place upon irradiation with a portion of UV light that is contained within sun light.
The term of photodegradation might be distinguished from photooxidation of the polymer. In the latter, oxygen is involved in the process while in the former light energy (E=hƲ) only is responsible for the photodegradation.
Mechanism of photooxidative degradation of polymers
Photooxidative degradation of polymers, which include processes such as chain scission, crosslinking and secondary oxidative reactions, and takes place via radical processes, similar to thermal oxidation reactions (Ranby and Rabek 1981; Carlsson et al. 1976; Mc Kellar & Allen 1979; Rnby and Lucki 1980).
Two mechanisms have been proposed to explain the photooxidation of polymers in conformity with similar observations made on low molecular weight compounds. One proceeds through direct reaction of singlet oxygen with the substrate while the other involves the production of radicals and subsequent reaction with oxygen (Geuskens & David 1979a 1979b; Trozzolo and Winslow 1968).
(I)The singlet oxygen mechanism of oxidation
(II)The free radical mechanism of oxidation
Steps of photodegradation
Initiation, propagation and termination.
This reaction may be initiated by physical factors such as: UV radiation, heat, ionization, ultrasonic or mechanical effects or by chemical factors (direct reaction with O2 or atomic oxygen, catalysis or singlet O2 [O2 *]1 excited state.
The “hydroperoxide” (POOH) is the most important initiator in the photooxidative process Grassie and Scott (1985).
The formation of hydroperoxide and its photolysis illustrate the formation of other effective functional groups such as carbonyl during β-scission of the alkoxy radical Grassie and Scott (1985).
There are many points concerning the mentioned propagation steps which are:
Formation of propagating radicals (POO.) by reaction (8), in a semi-rigid polymer system is very low (ca.1%) Mayo (1978) because of efficient polymer alkyl radicals (P.) recombination before O2 react with them. Polymer alkylperoxy radicals (POO.) are strongly resonance stabilized, and they are stable at room temperature in polymer matrix. They are selective electrophilic species abstracting 3° hydrogen in preference to 2° or 1° (Mill 1978; Guillet 1978Yousif et al. 2011b).
The light quanta produced by sun irradiation are energetically sufficient to cleave PO – OH and also P – OOH , but hardly POO – H bonds , which have the dissociation energies of 42 kcal/mol (PO – OH), 70 K cal/mol (P – OOH) , and 90 kcal/mol. (POO – H) Ranby and Rabek (1975b).The large differences in bond dissociation energy between PO – OH and P – OOH means that reaction with formation PO and OH radicals will predominate during light irradiation.
Polystyrene (PS) is a multipurpose polymer that is used in varied applications in rigid and foamed form. General purpose polystyrene is clear and hard which is used in packaging, laboratory ware, and electronics Meenakshi et al. (2002).
History of polystyrene
Edward Simon accidently discovered polystyrene in 1839 in Germany. From the resin of Turkish sweetgum tree, Liquidambar orientalis he obtained an oily substance, which thickened into jelly in air; he described it as styrol oxide. In 1845 John Blyth and August Wilhelm von Hofmann observed that the same changes occur in styrol in the absence of oxygen. They named it as metastyrol. Marcelin Berthelot in 1866 found that a polymerization process is responsible for the change styrol to metastyrol. In the thesis of Hermann Staudinger (1881–1965) it was reported that a chain reaction occurs in styrol resulting in the formation of macromolecules which was later called polystyrene. In Germany, I. G. Farben, company in 1931 started producing polystyrene in Ludwigshafen. The Koppers Company in Pittsburgh, Pennsylvania produced expanded polystyrene in 1959.
Synthesis of polystyrene
The reaction shown above has a heat of reaction of -121 Kj/mol (endothermic). Nearly 65% of all styrene is used to produce polystyrene.
Polystyrene is produced radical- initiated suspension polymerization. And some is produced by reactive extraction.
Types of polystyrene
Uses of polystyrene
Polystyrene is a type of plastic that is used for a variety of functions including in rigid items such as refrigerator crispers, coat hangers, DVD cases and printer cartridges. One of the important uses of PS is in the manufacture of cover signal lamps of some automobiles Safy Eldin and El-laithy (1994).
It is a brittle, high glass transition temperature polymer. Pure solid polystyrene is a colorless, hard plastic with limited flexibility which can be cast into molds with fine detail. Polystyrene is used in numerous plastic products. It is economical and is used for producing plastic model assembly kits, plastic cutlery, Fried (2003) for packaging and in sulation materials in the form of a foam or bead, and in electronics, construction, house and medical ware and disposable food services Meenakshi et al. (2002) and many other objects where a fairly rigid, economical plastic of any of various colors is desired.
Polystyrene fabricated into a sheet can be stamped (formed) into economic, disposable cups, glasses, bowls, lids, and other items, especially when high strength, durability, and heat resistance are not essential. A thin layer of transparent polystyrene treditimatly been used as an infrared spectroscopy standard. This is the lightweight material of which coffee cups and takeaway food containers are made. The voids filled with trapped air give expanded polystyrene low thermal conductivity. It is also used as insulation in the wall of building.
When a polymer matrix is mixed with inorganic nanoparticles, the thermal (Garcia et al. 2009), mechanical (Uhl et al. 2002), optical, electrical, magnetic and flammability properties of such a nanocomposite are much different from the polymer matrix itself Manzi-Nshuti et al. (2009).
Environmental effects of polystyrene
Synthetic plastics are used in many fields such as packing, household, agricultural, marine and architectural. Plastics have replaced natural resources such as cotton, wood and metals because of their light-weight, and durability. PS is a widely used thermoplastic. Its hardness, hydrophobic nature and chemical composition cause it to persist in nature without any decomposition for long period of time thus cause environmental pollution Singh and Sharma (2008). As waste plastic material has become a serious problem, recycling is receiving attention as a means of preserving the environment and reserving resources Pantano et al. (2009). Polystyrene waste requires the transportation of big large volume of materials, which is costly and makes recycling economically unfeasible.
Degradation of polystyrene
Polymers are weathered due to environmental factors such as light and temperature. The conditions of use play a key role in the degradation of plastics. Polystyrene losses its mechanical and tensile properties due to effect of UV light and heat Kiatkamjornwong et al. (1999). UV light induces the production of radicals by oxidation. Radicals cause the chains of polymer to breakdown.
Consumption of polystyrene in the world
Asia is the overall leader in production and consumption of polystyrene, with 53% of total world production and 47% of total consumption of polystyrene in 2010. North America and Western Europe follow distantly at about 17-19% of the total production and consumption each. Through the recession, the percentage of imports of EPS resin relative to consumption rose from 40% to 44% over 2007 through 2010. Global demand for polystyrene and expandable polystyrene increased from 13 mln tons in 2000 to around 14.9 mln tons in 2010. Packaging, construction, appliances and consumer electronics industries were the major consumers of polystyrene and expandable polystyrene.
The global demand for polystyrene and EPS is rising within developing countries such as China, India, Iran, Saudi Arabia and Brazil. Slovakia’s EPS consumption follows the trend set by other EU countries, whose year-on-year increase in consumption was about 3.3 percent during the monitored period. Of all EU countries, France, Poland, Austria and Germany reported the highest consumption of EPS. The lowest consumption was registered in Greece, Hungary, Italy and Spain. Complete insulation of a building using EPS can achieve a reduction of up to 66 percent in the heat consumption of prefabricated buildings, while in the case of detached family houses this can rise to as much as 70–79 percent. The life span of such insulation is about 50 years.
Photodegradation of polystyrene
Photodegradation of polystyrene in air causes discoloration (yellowing), cross-linking, and chain scission due to oxidation. A photodegradation process was also proposed on the basis of the IR spectrum of the photoirradiated film, which indicated the formation of peroxy radical and hydroperoxide intermediates. The photochemical reactions cause the dissociation of a polystyryl radical by creating an electrochemical excited state. The polystyryl radical is converted to peroxy radicals by reacting with oxygen. The peroxy radical undergoes chain scission and formation of carbonyl compounds.
Photooxidative degradation of polystyrene by radical processes
All commercial organic polymers degrade in air when exposed to sunlight as the energy of sunlight is sufficient to cause the breakdown of polymeric C–C bonds as a consequence of degradation. The resulting smaller fragments do not contribute effectively to the mechanical properties and the polymeric article become brittle. Thus the life of thermoplastics for outdoor applications becomes limited due to weathering Andrady et al. (1998).
When polystyrene is subjected to UV irradiation in the presence of air, it undergoes a rapid yellowing and a gradual embrittlement. Industrially, the yellow discoloration is an important adverse effect of the ageing of polystyrene, e.g. during exposure outdoors (Geuskens et al. 1978a 1978b; Weir 1978; Lucki and Rnby 1979; Rnby and Lucki 1980).
The main reactions observed are bond session, chain crosslinking and oxidative degradation. In spite of these great efforts the mode of photodegradation of polystyrene is still very controversial. A number of impurities and irregularities in polystyrene, such as hydroperoxides, aromatic carbonyl groups, olefin bonds and chain peroxide linkages, can be responsible for the photoinitiation of the radical oxidation of polystyrene Rabek (1987).
Irradiation of polystyrene by UV. and visible light with wavelength (λ< 400) nm., leads to the formation of radicals whose nature is dependent on the spectral composition of the light and irradiation condition Kuzina and Mikhailov (1993). The end group of PS or ketonic impurities also absorb the light of wave lengths longer than 300 nm (Geuskens and David 1979a 1979b; Klopffer 1975; George and Hodgeman 1977).
It has been suggested that the most important step in photolysis of polystyrene in the absence of oxygen is the scission of a C – H bond. The electron spin resonance (ESR) spectra obtained during the UV, irradiation of polystyrene (PS) were interpreted as arise from radicals formed in reaction (8) Cozzen and Fox (1969); Grassie and Weir (1965). The hydrogen radicals are very mobile; they can diffuse out from the polymer matrix and then recombine with each other to give molecular hydrogen.
The generally accepted theories of oxidation of polymers are based on the radical process for the thermal oxidation of hydrocarbons. This process involves peroxy group formation and it proceeds through the following fundamental steps Ranby and Rabek (1975a): initiation, propagation, radical chain branching and termination.
The type of the radicals formed during polystyrene photodegradation depends on the irradiation wavelength Ranby and Rabek (1975).
Photostabilization mechanisms in polymers
It is well known that all commonly used plastics degrade under the influence of sunlight. Almost all synthetic polymers require stabilization against the adverse effects; with the development of synthetic resins it became necessary to find ways and means to prevent, or at least reduce, the damage caused by the environmental parameters such as light, air and heat. That is why the photostability of polymers is one of the most important considerations for application.
Photostability can be achieved through the addition of special chemicals, light stabilizers or UV stabilizers, that have to be adjusted to the nature of the resin and the specific application considered.
The photostabilization of polymers involves the retardation or elimination of photochemical process in polymers and plastics that occur during irradiation. There are several different methods of photostabilization, and the choice of method is dependent on the polymer and application.The most important methods of photostabilization are the screening or absorbing of UV radiation by stabilizing agents and the use of antioxidants, which react with the polymer radicals, stopping the degradation process by forming inactive products (Ruoko 2012; Yousif et al. 2011a 2011b).
The following stabilizing systems have been developed which depend on the action of stabilizer: (a) light screeners, (b) UV absorbers, (c) excited state quenchers, (d) peroxide decomposers and (e) radical scavengers. Of these, it is generally believed that types c, d and e are the most effective Yousif et al. (2011a 2011b).
Practice shows that when the polymer contains a photostabilizer, the oxidation rate is much reduced. Stabilizers reduce but do not completely prevent oxidation, so it can be expected that some reaction will take place in the interior of a stabilized polymer.
Ultraviolet Stabilizers additives for plastics and other polymer materials which prevent the photodegradation or photocrosslinking caused by ultraviolet light.
The UV absorber and screener operate by absorbing the incident UV radiation preventing it from reaching the bulk of the polymer and converting the energy thus acquired into a less damaging form such as heat or they may act as radiation reflecting or scattering (preferably coating) Decker and Biry (1996) on the surface of the polymer thus delaying discoloration and delamination.
An important disadvantage of UV absorbers is the fact that they need a certain absorption depth (item thickness) to provide good protection to a polymer. Therefore, the protection of polymer surfaces and of thin items such as films or fibers is only moderate Gugumus (1987).
Thickness of the plastic.
Tolerance of color.
Effect of high concentration of absorber in plastics.
Compatibility of the absorber in the plastic.
The most common UV stabilizers are: UV absorber and light screeners, quenchers, hydroperoxide decomposers, radical scavengers and singlet oxygen, (1O2).
UV absorber and light screeners.
Singlet oxygen, (1O2), quenchers.
Rabek (The UV stabilizer can be classified into: 1987)
Hydroxy phenyl benzotriazoles.
Mode of action of UV. Absorber
The action of UV absorber is relatively simple, it interact with the first step of the photooxidation process, that is, it absorbs the harmful UV radiation before it reaches to the photo active chromophoric species in the polymer molecule (300–400) nm. Thus the energy dissipates in a manner that does not lead to photosensitization. A UV absorber must be light stable, because otherwise it would be destroyed in stabilizing reactions.
Certain phenolic and non-phenolic UV absorbers with structures (1), (2), (3) and (4) respectively, display high performance and inherent photostability in the (300–400) nm. region required for protection of polymers against photodegradation .The structure of some UV absorbers are shown in Figure 6: Pospisil and Nespurek (2000).
Generally, after photons are absorbed by the chromophores, molecules rise to higher excited state, by spin inversion of singlet state. The singlet states may change to triplet state by intersystem crossing (ISC) or return to a lower excited state by internal conversion (IC) (these are radiationless processes). Excited states have the ability to lose the excitation energy by some radiation processes such as fluorescence or phosphorescence or by energy transfer to another molecule.
Concerning the energy transformation in hydroxy benzophenones, it has been shown with 2-hydroxy benzophenone (Gugumus 1979; Allen 1983), that on exposure to light, it is transformed into the enol form which turns back into its initial form on losing thermal energy to the medium. On the basis of spectroscopic data, it is concluded that the energy transformation involves exclusively a fast radiationless transition.The photostabilizing process of O-hydroxy benzophenone has been the subject of many investigations Collell & Amer (1968). The most probable process involved is the utilization of the energy of the absorbed photon to intramolecular proton transfer during which a quinone structure is formed.
Excited state quenchers of chromophoric groups present in polymers.
The photostabilizing effect of many aromatic compounds to be UV stabilizer for several polymers has been reported. This is due to their filtrating action which depends in turn, on their absorption characteristics (Ranby and Rabek 1975; Heller 1969).
Pigments are insoluble inorganic or mineral and organic compounds of complex structure, such as:
Powder metal (aluminum) is excellent reflector to UV light.
Fe2O3, Fe3O4, ZnO,TiO2… are inorganic pigment excellent UV screener.
Organic pigments such as azo and anthraquenone display good UV light absorption.
Improving slip and skid resistance.
A pigment as a light screener should be
Light stable for long term performance without fading.
Heat stable to withstand polymer processing conditions.
Low cost and non-toxic.
The influence of pigments in polymer photostability is not completely understood. If an absorbing pigment is introduced into a polymer, it acts as an inner screen for photo products. If these products are not photooxidized, they accumulate in the polymer matrix. Since pigments act as highly absorbing additives, photooxidative phenomena will be limited mainly to the surface of samples Yousif (2012); Yousif (2010).
Carbon black contains different functional groups such as carbonyl, hydroxyl, quinone, ether, etc.…
Carbon black absorbs UV radiation more efficiently than conventional colored pigments, carbon black are efficient light stabilizers for polymers Winslow et al. (1969) such as polyethylene. Their high efficiency as light stabilizers is probably due to their ability to act as inner filters for UV radiation, and as radical scavengers, because many of the carbon blacks contain stable radicals Szwarc (1956), and quenchers of singlet and triplet states of polymers. The effectiveness of carbon blacks is dependent upon Williams et al. (1969) the type of carbon black, the particle size and the degree of dispersion in the polymer phase.
Thus the UV stabilization efficiency of carbon black increases as the particle size decrease. An optimum concentration of carbon black is 3-5%. Higher than this concentration, the polymer looses it tensile strength and other mechanical properties David and Hsuan (2003).
Energy transfer process.
Chemical and/or physical deactivation.
If energy transfer to the quencher can compete with reaction, decomposition… etc. by Ch, and if Q can dissipate the excess energy harmlessly, then the system is stabilized. Energy transfer can occur efficiently only if the energy level of the quencher is below that of the chromophore Lamolla (1969).
Long range energy transfer, e.g., a dipole/dipole interaction as is considered to operate between the chromophore and quencher even at distaices >50A if there is significant overlap between the emission spectrum of Ch and the absorption spectrum of Q Lamolla (1969).
Contact (collisional) energy transfer of various kinds is said to require that Ch* and Q be within 10 to 15. In practice, the quenching of excited triplets is usually ascribed to collisional transfer (Beavan and Phillips 1974; Dan et al. 1973).
In the solid state, transfer of energy occurs by conjugative or dipole-dipole interactions. The photooxidative degradation is promoted by the electronically excited oxygen molecule (singlet oxygen 1O2) formed in polymers. The [1O2] can also be generated in polymers by energy transfer from electronically excited carbonyl group to dissolved molecular oxygen Heskins and Guillet (1968).
The quenching of [1O2] is also necessary for effective stabilization. Nickel chelates have been proven to be very effective quenchers for the excited state of [1O2] Schmitt and Hirt (1963).
Intermolecular energy transfer
Intramolecular energy transfer
This process occurs within same polymer molecule, e.g. between an excited chromophore in the chain (donor) and another segment of the polymer molecule (acceptor). This process is especially interesting in co-polymers. Guillet (1972a 1972b).
Nickel chelates are very effective quenchers of the triplet state of carbonyl groups in polyolefins. These chelates have been tested for photostabilization of polyisobutylene, poly butadiene Lala and Rabek (1980), polystyrene George (1974), PVC, poly (2,6-dimethyl-1,4-phenyloxide) and poly urethanes. (Chandra 1983; Osawa et al. 1979).
Quenching of the excited state of carbonyl groups (ketones) through energy transfer.
Quenching of the singlet oxygen (1O2) Allen et al. (1984).
Decomposion of the hydroperoxides (OOH) radical, to non radical inactive species Yousif (2010).
Scavenging of radicals (alkylperoxy (ROO.) and alkyloxy (RO.) Allen et al. (1982).
These compounds operate by reacting directly with polymeric hydroperoxide (ROOH). The decomposition of hydroperoxide in polymer to non radical derivatives was first demonstrated Carlsson and Wiles (1974). Many metal complexes of sulphur containing ligands such as dialkylthiocarbonate and dialkylthiophosphate not only decompose hydroxide in PE film but are also effective in UV stabilization (as UV absorbers and excited state quencher).
Generally there are three groups of compounds which operate by quite distinct process Aliwi (2001).
Hindered amine peroxide decomposer
Hindered amine light stabilizers (HALS) have been found to be remarkably effective in performing both radical trapping and hydroperoxide decomposition.
These are one of the most effective photostabilizers for polymers and have been used in a large number of commercial polymers. They are efficient and cost-effective in many applications, despite their high prices Willis (1984).
The mechanism of (HALS) activity includes scavenging of R., ROO and deactivation of hydroperoxides (ROOH) and peracids, which are based on a complex of chemical transformations. Nitroxide the key intermediate formed from (HALS), is prone to scavenge alkyl and form O-alkylhydroxylamines Bagheri et al. (1982). Therefore HALS of different structure are able to interconvert in cyclic pathways, destroying species which could lead to polymer degradation and coating species which protect the polymer against degradation Willis (1984).
For the reaction of nitroxyl with (POOH) precedes via the formation of an intermediate (hydroxylamine) which reacts with (PO.) to generate the nitroxyl as reaction 3 as in Figure 31; Kurumoda et al. (1985).
Recently, different types of hindered amine light stabilizer have been synthesized to improve the compatibility of the additive with the polymer and enhance the long term of retention during the aging of polystyrene.
The scavenging of radical intermediates is another possibility for polymer stabilization, analogous to that used in thermal degradation. Quinones react with alkyl radicals to form radicals that do not initiate polymer oxidation.
Reaction with propagating radicals (P., PO. POO.).
Reaction with resulting hydroperoxides which are the source of chain branching through the propagating process (Feldman 2002).
Many reducing agents e.g. hindered phenols and aromatic amines, which reduce the ROO. to hydroperoxide in CB-D step have already been empirically selected and used for rubbers and by this time also for the newer plastics industry Cheremision (1997).
Photostabilization of polystyrene
The photostabilization process may be accomplished with commercial light stabilizers in addition to chalate complexes. The nature of the photostabilizer and polymer will determined the process and efficiency of photoprotection of the polymer film. The route by which photodegradation occurs and the importance of the impurities remaining after either polymerization or processing have to be known to determine the most satisfactory method of stabilization George (1974).
Two methods have been used to monitor the extent of photodegradation of polystyrene films. The first was by using FTIR spectra. The progress of photodegradation at different irradiation times was followed by observing the changes in carbonyl and hydroxyl peak intensities. Then, carbonyl (ICO) and hydroxyl (IOH) indices were calculated by comparison of the intensities of absorption peaks at 1720 and 3450 cm-1 with that of a reference peak at 1450 cm-1. This is called band index method. The second method involves measuring the average molecular weight using viscometry technique. These additives stabilize PS film through UV absorption or screening, and by peroxide decomposers, or radical scavengers Yousif et al. (2012).
Four methods have been used to monitor the degradation of polystyrene. There are: FTIR spectroscopy (measuring carbonyl and hydroxyl indexes), UV- visible spectroscopy, and solution viscosity (molecular weight). The last method for identification of degradation is by weight loss. The two anthraquinone derivatives and complexes provide good stabilization. Nickel and copper complexes provide better resistance to degradation than the uncomplexed anthraquinones Abd et al. (2009).
The protection of polystyrene films by UV absorbers including Ni(II) chelate complexes has been studied. Acetylactonate of Ni(II), Cu(II), and Co (III) complexes are more efficient than the corresponding Fe(III) complex for the photostabilization of PS. George (1974); Aliwi et al. (2001).
In recent years, the use of polymeric materials has rapidly increased but it is well established that rapid photodegradation of these materials is possible when they are exposed to natural weathering.
This review was talk about the photodegradation and photostabilization of polymers and especially in polystyrene. The “hydroperoxide” (POOH) is the most important initiator in the photooxidative process.
So most of the common polymers used in such applications contain photostabilizers to reduce photodamage and to ensure acceptable life times under outdoor exposure conditions. The photostabilization of polymers may be achieved in many ways. The following stabilizing systems have been developed, which depend on the action of stabilizer: light screeners, UV absorbers, excited-state quenchers, peroxide decomposers, and radical scavengers; of these, it is generally believed that excited-state quenchers, peroxide decomposers, and radical scavengers are the most effective.
However photoproduction will be enhanced if the additives can decompose –OOH, and possibly act as quenchers of some exited state in the early stages of the photodegradation
The authors acknowledge the Department of Chemistry, College of Science, Al-Nahrain University for their encouragement.
- Abd MA, Abdul Zahra AAI, Shenta AA: Photostabilization of polystyrene films by anthraquinones derivatives and their complexes with copper (II), oxovanadium (IV) and nickel (II) ions. Journal of Basrah Researches 2009, 35(3):81-97.Google Scholar
- Aliwi SM: Photostabilization of low density polyethylene for green house application. Nat J chem 2001, 2: 280-302.Google Scholar
- Aliwi SM, AL-Ani RR, Awad DAJ: Photostabilization of polystyrene films by Nickel and Copper tetradentate Shiff base complexes. Iraqi journal polymer 2001, 5(1):15-30.Google Scholar
- Allen NS: Photostabilising action of ortho-hydroxy aromatic compounds: A critical review. Polymer Photochemistry 1983, 3: 167-187.Google Scholar
- Allen NS, Chirinos-Padron A, Apployarat JH: Photo stabilization of PVC films by using some novel tetra Schiff's bases derived from1,2,4,5-tetra-[5-amino-1,3,4-thiadiazole-2-yl]-benzene. Polymer Degradation Stabilization 1982, 4: 223-228.Google Scholar
- Allen NS, Chirinos-Padron A, Appleyard JH: Polymer photodegradation: mechanisms and experimental methods. Polymer Degradation Stabilization 1984, 6: 31-37.Google Scholar
- Amin MU, Scott G, Tillekeratne LMK: Mechanism of the photo initiation process in polyethylene. Europ Polym journal 1975, 11: 85-126.Google Scholar
- Andrady AL: Advance Polymer Science.. 1997, 128: 49-94.Google Scholar
- Andrady A, Hamid S, Hu X, Torikai A: Effects of increased solar ultraviolet radiation on materials. Journal of Photochemistry and Photobiology B-Biology 1998, 46: 96-103.Google Scholar
- Ayako T, Hirose H: Advance Polymer Science. Polymer Degradation Stabilization 1999, 63: 441.Google Scholar
- Bagheri R, Chakraborty KB, Scott G: Mechanisms of antioxidant action: behaviour of a hindered piperidine and related oxidation products during processing and photooxidation of polypropylene. Polymer Degradation Stabilization 1982, 4: 1-9.Google Scholar
- Baloglu R, Fisch M: Polymer Degradation Stabilization. 1994, 45: 30-35.Google Scholar
- Beavan SW, Phillips D: Photostabilizing of macromolecule by excited state qyencher. Journal Photochem 1974, 3: 3149363.Google Scholar
- Blaga A: Durability of Building Materials and Compounds, ASTM STP 691. Edited by: Sereda PJ, Litvin GG. Philadelphia: ASTM; 1980:827-837.Google Scholar
- Bojinov VB, Grabchev IK: Novel functionalized 2-(2-hydroxyphenyl)-benzotriazole-benzo[de]isoquinoline-1,3-dione fluorescent UV absorbers: Synthesis and photostabilizing efficiency. Polym Photochem Photobiol 2005, 172: 308-315.Google Scholar
- Bottino FA, Di Pasquale G, Pollicino A, Recca A: Surface photostabilization of polystyrene by Tinuvin 1577. Journal of applied polymer science 1996, 69: 1251-1256.Google Scholar
- Bottino FA, Bottino G d P, Antonino P, Antonino R: Surface photostabilization of polystyrene by Tinuvin 1577. J of Appl Polym Sci 1999, 69(6):1251-1256.Google Scholar
- Bottino FA, Cinquegrani AR, Di Pasquale G, Leonardi L, Pollicino A: Chemical modification, mechanical properties and surface photooxidation of films of polystyrene. polymer testing. 2003, 12: 405-411.Google Scholar
- Bottino FA, Cinquegrani AR, Giovanna DD, Leonardi L, Antnino PA: Study on chemical modification, mechanical properties and surface photooxidation of films of polystyrene stabilized by hinderd amines (HAS), polymer testing. 2004, 23: 779-789.Google Scholar
- Carlsson J, Wiles DW: Physical properties of polymers handbook. J polym Sci, polym ChemEd 1974, 12: 2214-2217.Google Scholar
- Carlsson DJ, Garton A, Wiles DM: Macromolecules. 1976, 9: 695-701.Google Scholar
- Chandra R: Photostabilization of poly(2,6-dimethyl-1,4-phenylene oxide) by nickel(II)thiopicoline anilide. Polym Photochem 1983, 3: 367-378.Google Scholar
- Cheremision NP: Hand Book of Engineering Polymeric Materials, chapter 8. New York; 1997.Google Scholar
- Chirinos AJ: Mechanistic aspects of polymer photostabilization, j. photochem. Photobio. A:Chem 1989, 49: 1-39.Google Scholar
- Collell E, Amer J: Physiological and pathophysiological aspects of ceramide. J Chem. Soc. 1968, 90: 1012-1019.Google Scholar
- Cozzen RF, Fox RB: 12th Informal Conference on Photochemistry: proceedings of the 12th Informal. J Chem Phys 1969, 50: 1532-1540.Google Scholar
- Dan E, Somersall AC, Guillet JE: Macromolecules, New York. 1973, 6: 228-230.Google Scholar
- David SL, Hsuan YG: Assessing the photodegradation of geosynthetics by outdoor exposure and laboratory weatherometer. Geotextiles and Geomembranes 2003, 21: 111-122.Google Scholar
- Decker C, Biry S: Light stabilization of polymers by radiation cured acrylic coatings. Prog, Org coat 1996, 29: 81-87.Google Scholar
- Dindar B, Icli S: Unusual photo reactivity of zinc oxide irradiated by concentrated sunlight. J Photochemistry Photobio A: Chem 2001, 140: 263.Google Scholar
- Feldman D: Polymer weathering: photo-oxidation. Journal of polymer and the environmental 2002, 10: 163-173.Google Scholar
- Fried JR: Polymer science and technology. 2nd edition. New Jersey, Pearson Education, Inc: Publishing as Prentice Hall Professional Technical Reference.p; 2003. 359Google Scholar
- Galdi A, Foltis P, Shah A: UV protecting composition and methods of use. Application: US patent; 2010:2010-118415.Google Scholar
- Garcıa N, Hoyos M, Guzman J, Tiemblo P: Comparing the effect of nanofillers as thermal stabilizers in low density polyethylene. Polymer Degrad Stab 2009, 94: 39-48.Google Scholar
- Gardella JA: Characterization techniques for polymer blends. Appl Surf Sci 1988, 31: 72-102.Google Scholar
- George GA: Mechanism of photoprotection of polystyrene film by some ultraviolet absorbers. J Appl Poly Sci 1974, 18: 117-124.Google Scholar
- George GA, Hodgeman DKC: Polymer photodegradation: mechanisms and experimental methods. Eur polym J 1977, 13: 63-71.Google Scholar
- Geuskens G, David C: Degradation and Stabilization of Polymers. New York: Halsted, Wiley; 1975:113-127.Google Scholar
- Geuskens G, David C: Photooxidation of polymers a comparison with low molecular Wight compounds. Pure & Appi Chem 1979, 51: 233-240.Google Scholar
- Geuskens G, David C: Polymer photodegradation: mechanisms and experimental methods. Pure Appl Chem 1979b, 51: 233-240.Google Scholar
- Geuskens G, Baeyens-Volant D, Delaunois G, Lu-Vinh Q, Piret W, David C: Polymer photodegradation: mechanisms and experimental methods. J Europ Polym 1978, 14: 299-303.Google Scholar
- Geuskens G, Baeyyens-Volant D, Delaunois G, Lu-Vinh Q, Piret W, David C: Vacuum-ultraviolet photochemically initiated modification of polystyrene surfaces: morphological changes and mechanistic investigations. J Eur Polym 1978, 14: 291-297.Google Scholar
- Gijsman P, Diepens M: Photolysis and photooxidation in engineering plastics, Polymer Degradation and Performance. ACS Symp Ser 2009, 1004: 287-306.Google Scholar
- Goldshtein J, Margel S: Synthesis and characterization of polystyrene/2-(5-chloro-2Hbenzotriazole-2-yl)-6-(1,1-dimethylethyl)-4-methyl-phenol composite microspheres of narrow size distribution for UV irradiation protection. Colloid Polym Sci 2011, 289: 1863-1874.Google Scholar
- Grassie N, Scott G: Polymer Degradation and Stabilization. London: Cambridge University Press; 1985.Google Scholar
- Grassie N, Weir NA: Polymer photodegradation: mechanisms and experimental methods. J Appl Polym Sci 1965, 9: 975-981.Google Scholar
- Guaita M, Chiantore O, Costa L: Changes in degree of polymerization in the thermal degradation of polystyrene. Polymer Degradation stabilization 1985, 12(4):135-332.Google Scholar
- Gugumus F: Development in Polymer Stabilization-1. Edited by: Scott G. London: Applied Science Publishers Ltd; 1979:261.Google Scholar
- Gugumus F, Gachter R, Muller H (Eds): Plastics Additives. 2nd edition. Munich: Hanser; 1987:97-185.Google Scholar
- Guillet JE: Thermal characterization of polymeric materials. Polym Prepr Amer Chem Soc, Div Polym Chem. 1972, 13: 628-632.Google Scholar
- Guillet JE: Polymer photodegradation: mechanisms and experimental methods. Pure and ppl Chem 1972, 30: 135-144.Google Scholar
- Guillet J: Polymer Photophysics and Photochemistry. Cambridge University Press; 1985.Google Scholar
- Guillet TE, Ng HC: Macromolecules, Studies of the mechanism of polyolefin phorodegradation. Pure & Appi Chera 1978, 11: 929-935.Google Scholar
- Gupper A, Kazarian SG: Study of solvent diffusion and solvent induced crystallization syndiotactic polystyrene using FTIR spectroscopy and imaging macromolecules. 2005, 38(6):2327-2332.Google Scholar
- Hamid SH: Handbook of Polymer Degradation. New York: Marcel Dekker Inc; 2000.Google Scholar
- Heller HJ: Photochemistry of dyed and pigmented polymers. Eurp Polymer J Supplement 1969, 99-105.Google Scholar
- Heskins M, Guillet JE: Polymer photodegradation: mechanisms and experimental methods. Macromolecules 1968, 1: 97.Google Scholar
- Kaczmarek H, Kaminska A, Swiatek M, Sanyal S: Photoinition degradation of PS in the presence of low molecular organic compounds. European polymer Journal 1999, 36: 1167-1173.Google Scholar
- Kiatkamjornwong S, Sonsuk M, Wittayapichet S, Prasassarakich P, Vejjanukroh P: Degradation of styrene-g-cassava starch filled polystyrene plastics. Polym Degrad Stab 1999, 66: 323.Google Scholar
- Klopffer W: Polymer photodegradation: mechanisms and experimental methods. Eurpolym J 1975, 11: 203.Google Scholar
- Kochi JK, Wiley J: Handbook of Free Radical Initiators. J A Howard in Free Radicals 1973, 2: 3.Google Scholar
- Kurumoda T, Ohsawa H, Oda O, Fujita T, Toda T, Yoshioka T: Entropy and enthalpy effects of 4-(phenylthio)-substituted phenols. J Polymer Science Polymer Chemtry Ed 1985, 23: 1477-1482.Google Scholar
- Kuzina SI, Mikhailov AI: Plastics and the environment. Eur Polym J 1993, 29(12):1549-1589.Google Scholar
- Kuzina SI, Mikhailov A: Photocatalytic degradation of polystyrene plastic under fluorescent light. Eur Polym J 1998, 34: 291-320.Google Scholar
- Lala D, Rabek J: Polymer photodegradation: mechanisms and experimental methods. Polymer Degradation Stabilization. 1980, 3: 383-391.Google Scholar
- Lamolla AA: Energy Transfer and Organic Photochemistry, chapter 2. In Technique of Organic Chemistry. Edited by: Lamolla AA, Turro NJ. New York: Wiley; 1969.Google Scholar
- Lawrence JB, Weir NA: Polymer photodegradation: mechanisms and experimental methods. J Polym Sci Al 1973, 11: 105-431.Google Scholar
- Lucki J, Rnby B: Polymer degradation and stability. Pure Appi Chem 1979, 1: 1-6.Google Scholar
- Manzi-Nshuti C, Chen D, Su S, Wilkie CA: Structure–property relationships of new polystyrene nanocomposites prepared from initiator-containing layered double hydroxides of zinc aluminum and magnesium aluminum. Polym Degrad Stab 2009, 94: 1290-1297.Google Scholar
- Mayo FR: Long-term properties of polyolefins. Macromolecules 1978, 11: 492-496.Google Scholar
- Mc Kellar JF, Allen NS: Photochemistry of Man-Made Polymers, Ltd. London 306 S: Applied Science Published; 1979:138.Google Scholar
- Meenakshi P, Noorjahan SE, Rajini R, Venkateswarlu U, Crose S: Mechanical and microstructure studies on the modification of CA film by blending with Polystyrene. Indian Academy of Sciences 2002, 25(1):25-29.Google Scholar
- Mill TR, Richarason H, Mayo FR: J. Polym. Sci. Al. 1978, 11: 2899-2908.Google Scholar
- Olson DR, Schroeter SH: UV screen progenitors Thermally labile urethane derivatives of hydroxyphenylbenzotriazoles and hydroxybenzophenones. J Appli Poly Sci 1978, 22: 2165-2176.Google Scholar
- Osawa Z, Nagashima K, Ohshima H, Cheu E: Study of the degradation of polyurethanes the effect of various additives on the photodegradation of polyurethanes. J Polym Sci 1979, 17: 409-419.Google Scholar
- Pantano IAG, Diaz MF, Brandolin A, Sarmoria C: Mathematical modeling of the catalytic degradation of polystyrene in the presence of aluminum chloride. Polym Degrad Stab 2009, 94: 566-574.Google Scholar
- Patel P: Additive primer, blown films, cast films and extraction coating, PLACK conference. 2007, 16-20.Google Scholar
- Pinto L, Goi B, Schmitt C, Neumann M: Photodegradation of polystyrene films containing UV-visible sensitizers. Journal of Research Updates in Polymer Science 2013, 2: 39-47.Google Scholar
- Pospisil J, Nespurek S: Addcon World 2006. Prog Polymer Science 2000, 25: 1261-1335.Google Scholar
- Pospisil J, Habicher W, Zweifel H, Pilar J, Nespurek S, Piringer O: Polymer and polymer composites. AAA 2002, 10: 37-42.Google Scholar
- Pospisil J, Pilar J, Billingham NC, Marek A, Horak Z, Nespurek S: Factors affecting accelerated testing of polymer photostability. Polymer Degradation Stabilization 2006, 91: 417-422.Google Scholar
- Potts JE: Plastic environmentally degradation, The Kirk-Othmer Encyclopedia of Chemical Technology. 3rd edition. 1991. Supp. VolGoogle Scholar
- Pushpadass H, Weber R, Dumais J, Hanna M: Biodegradation characteristics of starch- polystyrene loose-fill foams in a composting medium. Bioresour Technol 2010, 101(19):7258-7264.Google Scholar
- Rabek JF: Comprehensive Chemical Kinetics. Volume 14. Edited by: Bamford CH, Tipper CF. Amsterdam: Elsevier; 1974:425.Google Scholar
- Rabek JF: Mechanism of Photophysical Process and Photochemical Reaction in polymers. New York: John Wiley and Sons; 1987.Google Scholar
- Rabek JF: Polymer photodegradation–mechanism and experimental methods. London: Chapman and Haal; 1993.Google Scholar
- Rabek JF: Polymer Degradation Mechanisms and experimental methods. Stocholm: Springer; 1994.Google Scholar
- Rabek JF: Polymer photodegradation-mechanisms and experimental methods. Cambridge: Chapman Hall; 1995.Google Scholar
- Rabek JF: Polymer photodegradation of polymers: physical characteristic and applications. Beelin: Springer- verlag; 1996.Google Scholar
- Rabek J, Ranby B: Studied on the photooxidation mechanism of polymers, photolysis and photooxidation of polystyrene. Journal of polymer science 1974, 12: 273-291.Google Scholar
- Rabek JF, Ranby B: Polymer photophysics and photochemistry: an introduction to the study of Photoprocess of macromolecules. J Polym Sci Al 1974, 12: 273-281.Google Scholar
- Rabek JF, Ranby B: Photodegradation, photooxidation and Photostabilization of Polymers. New York: John Wiley; 1975.Google Scholar
- Rabie ST, Mahran AM, Kamel EM, Abdel Hamid NH: Photodegradation of polystyrene stabilized with uracil derivative. Journal of applied sciences research 2008, 4(12):2015-2026.Google Scholar
- Ranby BG, Rabek JF: Photodegradation, Photooxidation and Photostabilization of Polymers. London: John Wiley & Sons; 1975:101-102.Google Scholar
- Ranby B, Rabek JF: Photodegradation, Photooxidation and Photostabilization of Polymers. Wiley periodicals, Inc; 1975b:165-184.Google Scholar
- Ranby B, Rabek JF: The effects of Hostile Environment on Coatings and Plastics. Edited by: Garnar DP, Stahl GA. ACS Washington, D.C: ACS Symp. Ser; 1981:291-301.Google Scholar
- Rnby B, Lucki J: New aspects of photodegradation and photooxidation of PS. Pure & Appl Chem 1980, 52: 295-303.Google Scholar
- Ruoko : Uv light induced degradation of polyethylene and polystyrene – spectroscopic and DSC study. Msc thesis: Tampere University of Technology; 2012.Google Scholar
- Safy Eldin NM, El-laithy SA: Photooxidative degradation of polystyrene of cover signals lamp of some automobile. Journal of applied polymer science 1994, 55: 47-54.Google Scholar
- Saitoh A, Amutharani D, Yamamoto Y, Tsujita Y, Yoshimizu H, Okamoto S: Structure and properties of the mesophase of syndiotactic polystyrene IV. Release of guest molecules from δ form of syndiotactic polystyrene by time resolved FT-IR and WAXD measurement. Polym J 2003, 35(11):868-871.Google Scholar
- Sampers J: Polymer Degradation Stablization.. 2002, 67: 455-463.Google Scholar
- Sastre R, Claramunt RC, Catalina FD, Mateo JL, Santa-Maria MD, Catalan J: Mechanism of photostabilization of polystyrene film by dihydroxyphenyl-pirazole. J polym Sci A; polymChem 1991, 28: 3661-3663.Google Scholar
- Sastre R, Catalina F, Mateo JL, Claremunt R, Santa-Maria MD, Catalan J: Mechanism of photostabilization of polystyrene film by dihydroxypirazoles. J of Polym Sci Part A: Polym Chem 2003, 28(13):3661-3668.Google Scholar
- Schmitt RG, Hirt RC: Handbook of hydroxybenzophenones. J Appl Polym Sci 1963, 7: 1565-1573.Google Scholar
- Schnabel W: Polymer Degradation: Principle and Practical Applications. Chapter 14. München: Hanser Int; 1981.Google Scholar
- Scott G: Green polymers. Polymer Degradation and Stabilization 2000, 68: 1-7.Google Scholar
- Senna M, Hamid H, Hussein M: Nuclear instrument methods. Phys Res Section B 2002, 187: 48-55.Google Scholar
- Shao Q, Wang L, Wang X, Yang M, Ge S, Yang X, Wang J: Hydrothermal synthesis and photocatalytic property of porous CuO hollowmicrospheres via PS latex as templates. Solid State Sci 2013, 20: 29-35.Google Scholar
- Singh B, Sharma N: Mechanistic implications of plastic degradation. Polym Degrad Stab 2008, 93: 561-584.Google Scholar
- Strlic M, Kolar J: Aging and stabilization of papers. Turjaška 1, 1000 Slovenia: Distributed by the National and university Library; 2005.Google Scholar
- Sun G, Jang H, Kaang S, Chae K: A new polymeric HALS: preparation of an addition polymer of DGEBA–HALS and its photostabilizing effect. Polymer 2002, 43: 5855-5863.Google Scholar
- Szwarc M: The action of carbon black in stabilizing polymeric materials. J Polym Sci 1956, 19: 462-589.Google Scholar
- Trozzolo AM, Winslow FH: Macromolecules. American chemical society publishing 1968., 98:Google Scholar
- Uhl FM, Wilkie CA: Polystyrene/graphite nanocomposites: effect on thermal stability. Polym Degrad Stab 2002, 76: 111-122.Google Scholar
- Valkoa L, Kleinb E, Kovarikb P, Simonb P: HPLC stanovenie sacharidov v procese modelovaného zrýchleného starnutia papiera. Eur Polym J 2001, 37: 1123-1133.Google Scholar
- Vinhas GM, Souto Maiora RM, Lapa CM, Almeida YMB: Degradation studies on plasticized PVC films submitted to gamma radiation. Mat Res 2003, 6: 497-500.Google Scholar
- Watson WF: Principles of polymer engineering rheology. Trans IRI 1953, 29: 29-32.Google Scholar
- Weidner S, Kuhn G, Freiedrich J, Schroder H: Plasmaoxidative and chemical degradation of poly(ethylene terepthalate) studied by matrix-assisted laser desorption/ionisation mass spectrometry. Rapid Communications in Mass Spectrometry 1996, 10(1):40-46.Google Scholar
- Weir NA: New aspect of photodegradation and photooxidation of polystyrene. Europ Polym J 1978, l4: 9-14.Google Scholar
- Wiles DM: Photostabilisation mechanisms in polymers: A review. Pure Appli Chem 1979, 50: 291.Google Scholar
- Wiles DM, Carlsson DJ: Photostabilisation mechanisms in polymers: A review. Polym Deg Stabil 1980, 3: 61-72.Google Scholar
- Williams FR, Jordan MW, Dannerberg EM: Reinforcement of elastomers by fillers: Review. J Appl Polym Sci 1969, 9: 861-871.Google Scholar
- Willis PB: Investigation of test method material properties and processes for solar cell in capsulation, eighth annual report. 1984.Google Scholar
- Winslow FH, Matreyek W, Trozzolo AM: Particle size distribution and morphology of in situ suspension polymerized toner. Amer Chem Soc Polymer Prepr 1969, 10: 1271.Google Scholar
- Wypych G: Handbook of material weathering. 4th edition. Toronto: Chemtec Publishing; 2008.Google Scholar
- Yousif E: Photostabilization of PVC by inorganic complexes. LAP LAMBERT academic publishing; 2010.Google Scholar
- Yousif E: Photostabilization of thermoplastic polymers. Germany: Lambert Academic Publishing; 2012.Google Scholar
- Yousif E, Salimon J, Salih N: New stabilizer for polystyrene based on 2-N-Salicylidene-5-(substituted)-1,3,4-thiadiazole compoundes. Journal of Saudia Chemical Society 2011a, 16(3):299-306. AGoogle Scholar
- Yousif E, Salimon J, Salih N: Photostability of poly (vinyl chloride). VDM Verlag: Dr. Muller publisher; 2011b. BGoogle Scholar
- Yousif E, Salimon J, Salih N: New stabilizer for polystyrene based on 2-Thioacetic Acid Benzothiazol complexes. Journal of applied polymer Science 2012, 125: 1922-1927.Google Scholar
- Yousif E, Hameed A, Salih N, Salimon J, Abdullah BM: New photostabilizers for polystyrene based on 2,3-dihydro-(5-mercapto-1,3,4-oxadiazol-2-yl)-phenyl-2-(substituted)-1,3,4-oxazepine- 4,7-dione compounds. SpringerPlus Journal 2013., 1–8:Google Scholar
- Zweifel H: Stabilization of polymeric materials. Springer-Verslag: Berlin Heidelberg; 1998.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.